Magneto-Optical Spectroscopy of Dilute Magnetic
Eric Chad Toppin Harley
A dissertation submitted to the faculty of the University of North Carolina at Chapel Hill in partial fulfillment of the requirements for the degree of Doctor of Philosophy in the Department of Physics & Astronomy.
Laurie E. McNeil, Advisor William W. Clark III, Reader John P. Hernandez, Reader Frank Tsui, Reader
Eric Chad Toppin Harley: Magneto-Optical Spectroscopy of Dilute Magnetic Semiconductors
(Under the Direction of Laurie E. McNeil)
Dilute magnetic semiconductors (DMS) are a class of semiconductors where a mag-netic ion has been randomly but substitutionally doped into a conventional semicon-ductor. DMS are currently envisioned as a key ferromagnetic material to be used in the construction of spintronic devices, or devices which operate based on the spin of spin-polarized charge carriers. I report primarily on magnetic characterization of Ga1−xMnxAs, and additionally on structural characterization of Ga1−xMnxN,
ex-amples of (III,Mn)V DMS. Magnetic Raman scattering experiments performed on Ga1−xMnxN were unsuccessful. Results from magnetic Brillouin light scattering (BLS)
measurements of Ga1−xMnxAs include the angular- and field-dependence of magnon
I would like to thank God for the opportunity to write this dissertation. The nature you have created is beautiful and mysterious; and I am grateful for the means and inclination you have given me to work at improving my understanding of a part of it, regardless how small.
You have brought many people into my life who have conspired to bring me to this point.
Ken Horst: thank you for introducing me to the wonders of science. Your enthu-siasm for chemistry and physics, your clear instruction, and your encouragement of creativity were all invaluable. I can’t imagine many high school science teachers would permit their students to build an apparatus, lash a model rocket engine to it, point the exhaust out the window, and press the ignition switch.
Carl Helrich, John Ross Buschert, Donald Clemens, Dan Smith, John Yordy, Doyle Preheim, Don Blosser, and other Goshen College professors: it is a rare thing to find so many people in one place who are both dedicated to teaching and so good at it that they make learning easy and enjoyable. You helped provide a solid educational background, and you also showed by example that education and faith needn’t be at odds with one another.
Laurie McNeil: through all the temptations for me to be sidetracked, you managed somehow to keep me pointed in the right direction. Thank you for putting up patiently with ever-slipping deadlines, for helpful advice, and for words of encouragement at opportune moments.
anyone else about the experiments I performed and the analysis of my results; without your help this dissertation truly would not have been possible.
Jacek Furdyna and Xinyu Liu at Notre Dame; Cammy Abernathy, Gerald Thaler, and others at the University of Florida: thank you for the generous provision of precious samples. I particularly want to indicate my appreciation for the time Dr. Liu took to converse via phone and email to answer additional questions.
William Clark and John Zavada: your monetary support not only made this project feasible, but also financed my education. Thank you.
Mom and Dad: thank you for all the support and prayers. I have always felt that you believed in my potential. You raised me to believe that I could do whatever I set my mind to, and without such encouragement I would likely never have attempted this degree.
David and Esther: thank you for accepting me into your family, and for opening your home so generously to mine. It has been a real blessing to have you so close this past year. Thank you for all the little and not-so-little ways you put our needs ahead of yours.
Becca, Noah, and Jadon: I owe you a greater debt of gratitude than anyone else, because this sometimes painful process has been hardest on you. Particularly in the past few months, Becca, you have had to act as a single parent while working full time. Noah and Jadon, you simply can’t understand right now why you don’t get to see your Daddy more than you do. One of the most difficult sacrifices for me to make while finishing my dissertation was giving up the special time I used to have with you. Now that I am finished, the thing I am most looking forward to is being able to spend time with my family once more.
LIST OF TABLES . . . . x
LIST OF FIGURES . . . . xi
Chapter I. Introduction . . . . 1
1.1 Progress in Information Processing . . . . 1
1.2 Electrostatic and Magnetostatic Interactions . . . . 3
1.3 Charge Carrier Polarization . . . . 5
1.4 Spintronics. . . . 5
1.5 Dilute Magnetic Semiconductors . . . . 8
1.5.1 II-VI DMS . . . . 8
1.5.2 III-V DMS . . . . 9
1.5.3 DMS and Spintronics . . . . 10
II. Materials. . . . 11
2.1 Ga1−xMnxAs. . . . 11
2.1.1 GaAs Host Crystal . . . . 12
2.1.2 Mn in GaAs . . . . 16
2.1.3 Ga1−xMnxAs as a DMS . . . . 18
2.2 Ga1−xMnxN . . . . 30
III. Structural Characterization of Samples . . . . 32
3.1 Raman Scattering . . . . 32
3.1.1 Raman Theory . . . . 32
3.2 Discussion of Structural Characterization . . . . 38
3.2.1 Ga1−xMnxN . . . . 38
3.2.2 Ga1−xMnxAs . . . . 49
IV. Magnetic Excitations in Crystals . . . . 51
4.1 Units in Magnetism . . . . 51
4.2 Classification of Magnetic Excitations . . . . 52
4.3 Calculation of Bulk Magnon Frequencies . . . . 53
4.3.1 Free Energy Density . . . . 54
4.3.2 Spherical Coordinates Method . . . . 56
4.3.3 Rectangular Coordinates Method . . . . 61
4.4 Damon Eshbach Solution . . . . 64
4.4.1 Boundary Conditions . . . . 67
4.4.2 Magnon Wavevector Relationships . . . . 69
4.5 Exchange Energy . . . . 71
V. Magnetic Characterization of Samples. . . . 75
5.1 Magneto-Optical Kerr Effect (MOKE) . . . . 76
5.1.1 MOKE Theory . . . . 76
5.1.2 MOKE Experimental . . . . 81
5.2 Magnetic Brillouin Light Scattering (BLS) . . . . 82
5.2.1 Magnetic BLS Theory . . . . 82
5.2.2 Magnetic BLS Experimental . . . . 83
5.3 Magnetic Raman Scattering . . . . 85
5.3.1 Magnetic Raman Theory . . . . 85
5.3.2 Magnetic Raman Experimental . . . . 86
5.4 Discussion of Magnetic Characterization . . . . 87
5.4.1 Magnetic Characterization of Ga1−xMnxN . . . . 87
5.4.2 MOKE Measurements of Ga1−xMnxAs . . . . 90
5.4.3 BLS Measurements of Ga1−xMnxAs . . . . 105
6.1 Ga1−xMnxN . . . . 120
6.2 Ga1−xMnxAs. . . . 121
VII. Appendix A: Simplification of the Exchange Energy Expression . . . . . 123
VIII. Appendix B: Direct Calculation of Fanis . . . . 125
LIST OF TABLES
2.1 Basic Materials Paramters for GaAs. . . . . 12
2.2 Angular momentum addition for strong spin–orbit coupling in the GaAs valence band. . . . . 14
3.1 Ga1−xMnxN samples, set A. . . . . 40
3.2 Ga1−xMnxN samples, set B. . . . . 45
3.3 Ga1−xMnxAs sample description. . . . . 48
4.1 Relevant Units in Electricity and Magnetism . . . . 52
5.1 MOKE loop fit results. . . . . 98
5.2 Anisotropy constants determined for sample 3.6. . . . . 111
LIST OF FIGURES
2.1 Zinc blende conventional unit cell.. . . . 13
3.1 Schematic phonon dispersion curve for GaN. . . . . 41
3.2 Raman spectrum of disordered Ga1−xMnxN, sample A5s. . . . . 43
3.3 Example of Ga1−xMnxN spatial inhomogeneity. . . . . 44
3.4 Raman comparison of Ga1−xMnxN sample set B. . . . . 45
3.5 Ga1−xMnxN defects vs. depth. . . . . 47
3.6 Typical Ga1−xMnxAs Raman spectra. . . . . 50
4.1 Spherical coordinates for calculating magnon frequency. . . . . 56
4.2 Calculating magnon frequency using spherical coordinates. . . . . 60
5.1 MOKE scattering geometries. . . . . 77
5.2 MOKE coordinate system. . . . . 80
5.3 MOKE experimental setup. . . . . 82
5.4 BLS experimental setup. . . . . 84
5.5 Magnetic Raman experimental setup. . . . . 87
5.6 Raman spectra of Ga1−xMnxN at 0 and 6 T. . . . . 88
5.7 MOKE loops from Ga1−xMnxAs samples 3.6 and 5.6. . . . . 90
5.8 Detail of easy and hard axis MOKE loops. . . . . 92
5.9 Calculated Fanis from hard axis MOKE loop. . . . . 96
5.10 Calculated hysteresis loops for sample 3.6 from hard-axis loop F extraction. 97 5.11 Fits of high-Happ portion of MOKE loops. . . . . 99
5.12 The effect of field cooling on MOKE loops. . . . . 102
5.13 Dependence of νmag on Mn concentration. . . . . 107
5.14 Evidence for surface magnon modes. . . . . 109
5.15 Angle and wavevector dependence for magnon modes in sample 3.6. . . . . 112
5.16 Angular variation of F in the plane for sample 3.6. . . . . 114
B.1 Excel worksheet layout for calculating Fanis. . . . . 125
B.2a Excel Visual Basic code for calculating Fanis directly, page 1/4. . . . . 126
B.2b Visual Basic code, page 2/4. . . . . 127
B.2c Visual Basic code, page 3/4. . . . . 128
Progress in Information Processing
Over the last half of the twentieth century, automated numerical computation rev-olutionized both scientific research and our daily lives. It became possible to explore analytically intractable problems and solutions; and with each increase in the speed of computers, a new level of sophistication in calculations became possible. The com-puter, originally an incredibly bulky, expensive device, seemingly only of interest and use to researchers, became smaller, less expensive, and faster. Si-based integrated cir-cuits, the workhorse of modern computers, are ubiquitous in today’s modern societies, finding use in applications as varied as air traffic control systems, automobiles, toast-ers, and greeting cards. Improvements in design and production of these integrated circuits have resulted in such a steady increase in performance (as a consequence of decreasing size and power consumption per calculation) that this increase has been codified as Moore’s Law [[1–3]].
electronic configuration, and as such provides the framework in which charge transport in a semiconductor can be understood. Spatially-targeted modification of the band structure via doping with electrically active impurities creates active electronic devices embedded in the semiconductor crystal. These individual devices are connected and organized on a very large scale (VLSI, very large scale integration) to produce modern integrated circuits.
One of the dominant contributions to the steady increase in performance of in-tegrated circuits has been a steady decrease in the size of chip features. Since chip functions depend on transporting charge from one location to another, decreasing feature size has the benefit of decreasing the amount of charge that must be moved as well as decreasing the distance it must travel. These factors allow operations to consume less power and proceed more rapidly. As was inevitable, chip features, now as small as tens of atoms in some cases, are reaching fundamental physical limits; so further improvements in performance must increasingly come from sources other than from simply shrinking the architecture. A significant additional complication is the fact that at such small scales quantum mechanical effects can no longer be neglected. Two general strategies remain for improving information processing technology []:
1. Redesign within the context of classical electronics. Approaches include devel-opment of new materials with improved properties, coupled with modification of device design and modification of integration schemes.
2. Step outside the limits of classical electronics. Design devices that actually make use of quantum effects in order to surpass current technology.
is a more fundamental change means that there is also the possibility that it will produce much larger improvements. Spintronics is one such area of research, where some commercially successful devices have already been made, and where many hope that future advances will change the operating principles of many integrated circuits entirely.
Electrostatic and Magnetostatic Interactions
Before delving into any details of spintronics, it is instructive to perform a brief comparison of the way that a particle such as an electron interacts with its environment via its charge and via its spin. This comparison should serve not only to highlight some physical reasons for differences between the historic development of electronic devices (transistors, integrated circuits) and magnetic devices (typically information storage), but it should also serve as a reminder of the inherent richness and complexity of magnetic phenomena.
A charge interacts with its environment via the electric force, which is both very long-range and strong. In fact, the potential energy associated with electrostatic interactions between two point charges only drops off as ∼ |
−1 with distance. For a
semiconducting material such as GaAs, which has a static dielectric constant of 12.9 [], a system of two elementary charges brought to a separation of 0.5 nm will have a potential energy of magnitude 0.2 eV, or 4?10−20J. Small voltages (either intentionally
applied or as a result of stray fields) also have a large effect on the potential energy of an elementary charge, where by definition moving the charge through a potential of 1 V changes the energy of the charge by 1 eV, or 1.6?10−19 J.
regions of integrated circuits over long periods of time. The strong mutual repulsion experienced by like charges means that such an arrangement is necessarily a local rather than a global energy minimum, and the charge (voltage) state tends to decay over time, even if through no other effect than tunneling. Even small stray electric fields can also cause significant difficulties with the operation of integrated circuits.
The dipole-dipole magnetic interaction between a pair of spins is both smaller in magnitude (∼10−25J≈10−7 eV for a separation of 0.5 nm) and has a shorter range (∼ r−3) than the electrostatic interaction above. Similarly, the potential energy of a spin
in a magnetic flux density as high as 1 T is only∼10−24 ≈10−4 eV; so there are easily
5 orders of magnitude between magnetic dipole-dipole interactions and magnetostatic interactions. The short range means the difference will only increase with separation between spins/charges. Clearly spin orientation is less likely to be disturbed by stray magnetic fields than electric charge position is to be disturbed by stray electric fields. In information storage applications, the short range and weakness of this magnetic dipole-dipole interaction allows for high storage densities: small magnetic “bits” can be in close proximity and still remain independent, each unaffected by the other’s magnetic field.
The dipole-dipole magnetic interaction is weak enough that it cannot account for magnetic ordering in materials: a material with TC of ∼100 K has magnetic
interac-tions operating on an energy scale of kB?100 K = 1.4?10−21 J≈10−2 eV. However,
symmetry requirements and the Pauli exclusion principle when particles with spin have overlapping spatial wavefunctions, appearing for example as the energy splitting between singlet and triplet states. Once the exchange interaction sets up a magnetic ground state, spin-orbit coupling shows up as magnetocrystalline anisotropy. This magnetocrystalline anisotropy is responsible for defining a preferred orientation for the average magnetization of the crystal.
Charge Carrier Polarization
So far I have described ferromagnetic effects implicitly in the context of localized lattice spins. Such lattice spins in a ferromagnet spontaneously align parallel to each other, due to the exchange interaction. This alignment of the lattice spins and the exchange interaction also have an effect on the charge carriers present in the material. While a material with no net magnetic moment typically has equal numbers of spin-upn↑ and spin-down n↓ charge carriers, a material with a net magnetic moment does
not. One then speaks of the percent polarization of the charge carriers, calculated as 100%? (n↑−n↓)/(n↑ +n↓). Although Zeeman splitting can contribute to this
polarization, in ferromagnetic materials in the presence of small applied fields the most important contribution to the net spin polarization of the charge carriers is the exchange interaction. The band structure of ferromagnetic crystals, when plotted separately for each spin orientation, displays the resulting spin polarization as an imbalance in the density of states at the Fermi level. There are simply more available low-lying electronic states for a particular spin orientation.
While the termelectronics where devices operate based on electric charge, spintronics
refers to research with the end goal of producing devices which function based on the spin of their charge carriers. The subject, of course, existed before the buzzword, and is generally agreed to have started in 1988–1989 with the discovery of GMR (giant magneto resistance) by groups led by Fert [] and Gr¨unberg []. Although researchers had been aware that the spin polarization of a sequence of ferromagnetic layers could affect the resistance of a current traveling through them, this was the first time such an effect had been obtained with a useful magnitude and at useful temperatures [].
Awschalom et al. [] divide spintronic devices into three classes, which will here-after be referred to by their numbers.
1. Devices in which spin-polarized currents travel in ferromagnetic metallic alloys.
2. Devices in which spin-polarized currents travel in semiconductors.
3. Devices that use individual electron spin for quantum computations.
The first two classes of spintronic device are in principle much simpler to realize, since they involve manipulating charge carriers in bulk and should not require as fine control on such a small scale. Devices of class 1 were the first to be developed, simply due to the ready availability of metallic alloys that are ferromagnetic at room tempera-ture. The first commercially successful spintronic device is the GMR (giant magneto-resistance) read head for HDD’s (hard disk drives); MRAM (magnetic random access memory) is expected to follow next.
magnetization of the unpinned layer is reversed relative to the pinned layer, charges from one layer scatter more when they cross over into the layer with opposite spin orientation, increasing the measured resistance of the read head. The GMR effect allows one to make HDD read heads that are much more sensitive than the previous MR (magneto-resistance) read heads, permitting a reduction in size and magnetic field of magnetic bits on the HDD. This reduction in size and field of the magnetic bits has generated a huge increase in storage density for the HDD’s, accompanied by an increase in data transfer rates.
While spintronic devices of the class 1 are clearly useful, they have thus far been limited to improving the performance of existing devices. Much more exotic develop-ments are expected if and when spintronic devices of class 2 are produced. For this class of devices, spin-polarized currents could either be injected from a metallic fer-romagnet into the semiconductor, or a magnetic semiconductor could be used as the source of the spin current. Achieving successful spin current injection into a semicon-ductor would allow all the existing expertise in semiconsemicon-ductor devices and integration to be brought to bear on the field of spintronics.
The SFET (spin field effect transistor), first proposed by Datta and Das in 1990 [], has become the prototypical spintronic device, and falls into Awschalom et al.’s class number 2. A spin current is injected into the channel of an FET (field effect transistor) with ferromagnetic source and drain. If a gate voltage is turned on, the spin current precesses in the presence of the applied electric field; when the spin current reaches the ferromagnetic drain, its orientation relative to the magnetization direction of the drain determines the magnitude of the current. It is typically thought that such an arrangement could provide speed and power consumption improvements over traditional FETs, as well as novel functionality such as logic gates whose functions can be changed at will [].
the trip from the ferromagnetic source into the channel, and then from the channel into the drain. While spin current injection from metals into semiconductors has proven difficult [], one may be able to sidestep many of these difficulties by designing semiconductors with magnetic properties.
Dilute Magnetic Semiconductors
DMS (dilute magnetic semiconductors, often also referred to as diluted magnetic semiconductors orsemimagneticsemiconductors) are considered to be good candidates for creating spintronic devices of class 2. A DMS can be defined as a semiconductor into which a magnetic ion has been substitutionally doped, occupying random lattice or sublattice positions in the host. In practice, this “doping” must occur at very high levels (generally from 1% to nearly 90% substitution in some materials) so that enough magnetic ions are present to result in a magnetically-ordered ground state.
If one can achieve aferromagnetic DMS with only relatively minor changes in band structure from the undoped semiconductor host, then spin currents in semiconductors, essential for the class 2 spintronic device, may be easier to achieve. Furthermore, there is some hope that the material growth or doping could be incorporated into integrated circuit production in a straightforward manner, allowing efficient scale-up. The primary technical difficulty has been in raising TC, the Curie temperature.
DMS were not originally conceived for the purpose of implementing spintronics They were first studied in great detail in the 1980s [[11–13]], as basic materials re-search into their unique semiconducting and unique magnetic properties. Ternary AII
1−xMnxBVI compounds such as Hg1−xMnxSe, Cd1−xMnxTe, and Zn1−xMnxTe were
in these AII
1−xMnxBVI compounds, ranging from 0.38 for Hg1−xMnxSe all the way up
to 0.86 for Zn1−xMnxTe []. This high solubility of Mn, higher than that of other
transition metals, was typically ascribed to the special 4s2 3d5 electronic
configura-tion []. While other transiconfigura-tion metals had the same completely filled s shell, the half-filled d shell of Mn was especially stable, causing the Mn to act much more like a group-II element.
Despite the success in understanding these AII
experimen-tally and theoretically, they have proven unsuitable for practical spintronic applica-tions. Not only is Tcrit, the transition temperature below which spontaneous magnetic
ordering appears, too low; but also these DMS to do not typically exhibit ferromag-netism. Instead they form spin glass or antiferromagnetic states at low temperature, depending on x. Antiferromagnetic states and spin glass states cannot contribute to uniform spin polarization of charge carriers throughout the crystal: spin glasses don’t exhibit long range magnetic order; and antiferromagnets, although exhibiting long range order, have equal numbers of lattice spins pointing up and down.
A natural extension to the early work on DMS, which had focused mainly on II-VI (and to a smaller extent on IV-VI and II-V) compounds [], was to try to make a DMS based on III-V materials. Growth of the first III-V DMS, In1−xMnxAs, was first reported
in 1989 by Munekata and Ohno et al. [] and reviewed by Ohno and Munekata et al. [] in 1991. Magnetic ions in III-V semiconductors had previously been limited to 1025 m−3, which for Ga
1−xMnxAs would correspond to x = 5 ?10−4, but
low-temperature MBE growth (less than 300◦C) opened the door to growth of compounds
with magnetic ion content two full orders of magnitude higher. In1−xMnxAs was first
reported with x as large as 0.18, and the magnetic properties were later shown to depend on growth conditions and carrier type and concentration.
In the early 1990s most III-V DMS research involved In1−xMnxAs; but in 1996
DMS Ga1−xMnxAs, achieving single-phase material via LT-MBE, with x as high as
0.07. This was an important development, since GaAs is the most well-understood and widely-used III-V compound; researchers hoped that the existing body of knowledge on the properties and growth of GaAs would facilitate understanding of this GaAs-based DMS.
DMS and Spintronics
The first reported growth, in 1989, of III-V DMS followed very closely on the heels of the discovery of GMR [], which is widely held to be the start of spintronics []. However, it was not until Ohno et al.’s Ga1−xMnxAs paper in 1996 [] that explicit
mention was made in DMS literature of spintronics as a justification for studying DMS. Many other DMS papers published in the same and subsequent years made at most passing reference to potential technical utility in their introductions [[18–22]]. Although it seems likely that potential spintronics applications were in the back of researchers’ minds as they studied III-V DMS, their primary motivation was still one of basic materials properties research. III-V DMS were basically the newest vehicle for the interesting effects that appeared in this intersection between semiconductors and magnetism [[11, 21]].
The current motivation for studying III-V DMS is almost entirely advancement of the field of spintronics. The most fundamental barrier to the creation of practical spintronic devices using DMS is producing a DMS with sufficiently high TC: TC must
be at or above room temperature. The use of Mn as the magnetic dopant in the first III-V DMS, In1−xMnxAs and Ga1−xMnxAs, may largely have been a carryover from its
successful incorporation in II-VI DMS. It was also known, though, that Mn has the lowest ionization energy of 3d transition metals in GaAs, which means that according to a general rule of thumb, it should have the highest impurity solubility []. Some currently hold the opinion that although the Ga1−xMnxAs TC has not yet exceeded
room temperature, there is no fundamental limitation preventing it from doing so []. Ga1−xMnxAs is the most mature III-V DMS, having been studied actively since
its first reported growth in 1996 in a collaboration between Tohoku University and University of Tokyo researchers Ohno et al. []. Mn had previously been studied as both an unintentional and intentional impurity in GaAs [[26, 27]], but due to its low solubility in GaAs had never been incorporated in large enough quantities to qualify as a DMS.
Table 2.1: Basic Materials Parameters for GaAs. After Blakemore [].
Parameter Value Units Comments
a 5.65325?10−1 nm measured at 300 K rc-c 2.44793?10−1 nm
3a/4, nearest neighbor distance
Vcell 1.80674?10−1 nm3 a3, conventional unit cell volume Vcell 4.45168?10−2 nm3 1
4a3, primitive cell volume
of Ga1−xMnxAs at higher x than would otherwise be possible, by limiting the
mobil-ity of Mn during the growth process. If growth temperatures are much greater than 250◦C the Mn can reorganize and precipitate as secondary phases such as
ferromag-netic MnAs [], which has a TC of 310 K. The first reported growth by Ohno et al.
incorporated Mn with x ranging from 0.015 to 0.07, with the highest measured TC of
60 K for the x = 0.035 sample. Conductivity was determined to be p-type. Ohno et al. also proposed that the observed in-plane easy axis could result from the biaxial compressive strain in the Ga1−xMnxAs layer. In1−xMnxAs epitaxial layers were
deter-mined to have an out-of-plane easy axis, but they were under biaxial tensile strain.
GaAs Host Crystal
It would certainly be futile, and at any rate would not suit my present purpose, to try to improve upon Blakemore’s excellent review [] of GaAs properties published in 1982 in theJournal of Applied Physics. I will reproduce some of the relevant GaAs materials properties here.
Figure 2.1: Zinc blende conventional unit cell. Some common lattice vectors are labeled. Observe that although this lattice has cubic symmetry in bulk, when the lattice terminates at the surface of a crystal the  and £110¤ directions are no longer equivalent.
cubic (fcc) sublattices, offset by a vector of £1 4,14,14
Table 2.2: Angular momentum addition for strong spin–orbit coupling in the GaAs valence band.
l s j mj Designation
2 l+s= 32 ±32 heavy hole band
2 light hole band
2 ±12 split-off band
Electronic Band Structure
GaAs has a direct band gap of 1.42 eV at 300 K []. The two highest valence bands consist of the Γ8 “heavy hole” band, with lower dispersion near zone center, and the Γ8
“light hole” band with higher dispersion near zone center. These bands are degenerate at Γ(000), split because of the difference in dispersion at small crystal momentum
k, after which the bands run almost parallel for larger k. This nonparabolicity is also a characteristic both of the Γ6 conduction band and of the third-highest valence
band, referred to as the spin split-off band. This band has symmetry Γ7 and lies
approximately 0.341 eV below the Γ8 valence bands’ peaks.
The basic splitting scheme at the zone center for these three highest-energy valence bands can be understood by coupling the orbital angular momenta of the p orbitals directly to the spin of the charge carriers, due to a strong spin–orbit interaction []. See Table 2.2, page 14. In p-type material this leaves us with a majority of charge carriers that are holes with total angular momentum j = 3
2. In the literature this
total angular momentum j is sometimes referred to as effective spin, and even more confusingly, merely as spin.
Although the parabolic heavy hole band has a much higher density of states near the Fermi level than the other valence bands, for sufficiently high hole density ρh
Ga1−xMnxAs, showing up in seemingly unexpected and macroscopically significant
ways. For example, if only one hole band were occupied in Ga1−xMnxAs the observed
compressive strain ↔ in-plane magnetic easy axis and tensile strain ↔ out-of-plane easy axis relationships would be reversed entirely [].
Defects in GaAs
While knowledge of fundamental properties of semiconductors such as the symme-try of the crystalline lattice, the nature of the bonding, and electronic band structures, is certainly a prerequisite for understanding materials properties, in many cases defects actually dominate the measured properties of real samples. Although this domina-tion complicates the study of materials, especially in the early stages, the controlled introduction of defects is the founding principle of virtually all semiconductor-based electronics and optics []. Weber [] gives a very readable overview of defect classi-fication and provides short narratives of the historical development of understanding of certain defects in some of the more technologically important semiconductors. No-tably, Weber refers to the so-called EL2 (electron level 2) defect in GaAs which has been determined to be related to the As antisite defect AsGa [[32–38]]; and he refers to
the mysterious n-type background dopant in GaN that was widely assumed to be a N vacancy VN but instead turned out to be a substitutional O impurity ON [[39, 40]].
The notation for defects is defectlocation, so that AsGa stands for an arsenic atom on a
Low-temperature growth techniques, such as low-temperature molecular beam epi-taxy (LT-MBE), are employed instead when one wants to achieve nonequilibrium
growth of a material. LT-MBE growth is what enabled the incorporation of Mn into III1−xMnxV at concentrations high enough to produce DMS []. LT-MBE had
previ-ously been used to grow GaAs, and, these results can provide some insight into the kinds of non-Mn-related defects that should be present in Ga1−xMnxAs.
GaAs LT-MBE growth is carried out between 200 and 300◦C [[41, 42]], consistent
with Ga1−xMnxAs growth conditions. Structural properties have been studied with
XRD [[41,42]], and specific defects have investigated using optical absorption techniques as well as EPR and STM, according to Liu et al. [] and references therein. These structural and electronic data show that defects in LT MBE GaAs are mainly As antisites AsGa (substitution of Ga by As) and Ga vacancies VGa. The amount of As
interstitals AsI is negligible [].
It is observed that as the growth temperature is decreased, the stoichiometry shifts towards As, so that for lower growth temperature there is a higher incidence of AsGa
and [[41–43]]. By far the most plentiful defect, and responsible for the observed con-ductivity [], is GaAs, with VGa playing a supporting role by compensating some of
the AsGa donor defects []. The AsGa alone is also found to account for the large
lattice expansion [].
Mn in GaAs
Ohno et al.’s reported growth of Ga1−xMnxAs [] was not the first time GaAs
had been doped with Mn. In fact the same group, in their 1989 Physical Review Letters article [] announcing the growth of the first III-V DMS (In1−xMnxAs), also
mentioned the growth of Ga1−xMnxAs via LT-MBE. Although they reported
ferromag-netic behavior, they did not report the amount of Mn incorporated, and their substrate temperature of 400◦C implies the presence of secondary phases in the Ga
At any rate, little if any mention seems to have been made of Ga1−xMnxAs
to take their claim in the 1996 paper, of the first growth of the ferromagnetic DMS Ga1−xMnxAs, additionally as confirmation that the 1989 Ga1−xMnxAs sample was not
a true (substitutional) DMS.
Before the advent of III-V DMS through nonequilibrium LT-MBE growth [], Mn was studied as both an unintentional and an intentional dopant of GaAs. Almeleh and Goldstein performed EPR measurements in 1962 [] on GaAs intentionally doped with Mn up to a concentration of 1023–1024 m−3, or x≈10−5. They reported that it
behaved as an acceptor, that its activation energy for diffusion in GaAs was 2.75 eV, and that these observations were consistent with the logical expectation that Mn should substitute for Ga.
Klein [] documented Mn as a trace element in bulk GaAs, and noted that it mi-grated to the surface upon heat treatment of 90 minutes to 24 hours at 1010 K. While this is much higher than the 450–500K annealing temperatures used for Ga1−xMnxAs,
that was necessary for sufficient mobility of the MnGa. (By contrast, in annealing
a Ga1−xMnxAs sample one would prefer the MnGa to be completely immobile, and
instead only drive out the MnI.) In that work, a photoluminescence (PL) band
ob-served at 1.41 eV PL band was assigned definitively to the MnGa. The Mn depth
profile as measured by SIMS, started at 6?1023 m−3, or x≈ 3?10−5, at the surface
and dropped to much less than 1023 m−3 in the bulk. By means of comparison, an
intentionally-doped reference sample had a Mn concentration of 4.9?1023 m−3, which
would correspond to x= [Mn]a3/4 = 2?10−5 in Ga
1−xMnxAs, much lower than the
typical DMS range ofx≈0.01–0.1.
Another example of growth of such samples is found in a 1987 paper [] by Schneideret al.on ESR of Mn in GaAs. This GaAs:Mn was grown via the Czochralski technique, with the Mn dopant introduced during crystal growth. SIMS showed the Mn concentration to be 1023 m−3, or x ≈ 5?10−6, while the material was weakly
As as a DMS
As mentioned earlier in section 1.5.2, nonequilibrium LT-MBE growth was the key to the incorporation of substitutional Mn in concentrations high enough for the Ga1−xMnxAs to be considered a DMS, typically x & 0.01, or [Mn] & 2?1026 m−3.
This is an extremely high doping level, and really falls into the range that many would term “alloying” rather than “doping.” Efforts have proceeded on many fronts, both experimental and theoretical, to understand and optimize this DMS. While the pri-mary goal of much of the experimental work has been the yet-unrealized achievement of useful room temperature ferromagnetism, an enormous amount of additional knowl-edge has been amassed along the way. While MnGa is not considered a defect in the
context of Ga1−xMnxAs (in fact it is the desired location of the Mn), it is a defect in
the traditional sense and in the context of the host crystal GaAs. As such it disturbs the symmetry, lattice constant, charge distribution, carrier density, and overall band structure of the GaAs by its presence; and all of these factors play important roles in the observed ferromagnetic properties.
The interplay between experiment and theory is perhaps especially important in a developing subject area like III1−xMnxV DMS research. Theorists need experimental
confirmation of results to tell them which approximations and calculation schemes are appropriate. Experimentalists also need to compare results with theoretical cal-culations to understand the often bewildering array of results that arise in a material whose significant properties depend on subtle details of what are essentially defects. Therefore, even with a goal of understanding the basic properties of Ga1−xMnxAs
that are observed in experiment, an appropriate place to start is an extensive re-view of III1−xMnxV DMS theory by Jungwirth, Sinova, Masek, Kucera, and
MacDon-ald [], to be published inReviews of Modern Physics, but also available on online at
Journal of Magnetism and Magnetic Materials in 1999 [], to see just how much the field has advanced in seven years.
Mn Incorporation in Ga1−xMnxAs
MnGais responsible for the ferromagnetic properties of Ga1−xMnxAs, and it
accom-plishes this in two ways. Since its electronic configuration is [Ar]4s23d5, the electrons
in the half-filledd shell have their spins aligned, for a large spin of 5/2. The half-filled
d shell acts almost like a filled orbital, leaving the 4s2electrons as the easiest to ionize,
and causing the Mn to act chemically very much like a Group-II element. Therefore in Ga1−xMnxAs as MnGa (sitting on a Group-III site) it acts as an acceptor. MnGa
turns out to be the most stable position for Mn in the GaAs lattice, so it is also the most common position []. We can describe possible charge states of this acceptor as follows [[24, 27, 46]].
1. A0(3d4) The neutral Mn
Ga acceptor, A0, in the tight-binding limit, is one where
it has contributed three electrons to the valence band, since it is sitting on a Group-III lattice site.
2. A−(3d5)The 3d5electron configuration corresponds to the ionized acceptor state,
since in this case the MnGais contributing only two electrons to the valence band.
3. A0(3d5+hole) An alternative neutral state to the tight-binding limit of A0(3d4)
is to retain the stable 3d5 core and then have a loosely-bound hole in a large
effective mass orbit.
The binding energy for the hole in A0 has been consistently measured as∼0.11 eV
over the years [], but was unclear for some time which of the twoA0 states actually corresponds to the ground state of Mn in GaAs (see [[24, 27, 48–50]] and references therein). The presence to some degree of bothA0 states has been conclusively demon-strated by direct STM imaging of the A0(3d5+hole) state [[51–53]] and by spin-flip
assert that the A0(3d4) should provide an important contribution to the observed
ferromagnetism, it seems that current theoretical methods adequately describe the ferromagnetism without taking A0(3d4) into account. In fact, not the neutral ground
state but the ionized acceptorA−is by far the most common state for Mn to be found in throughout the range of Mn and experimental conditions of interest, due to the metal-insulator transition at high Mn concentrations [].
Local and Itinerant Magnetic Moments: The Nature of Ga1−xMnxAs
Knowing the nature of the Mn acceptor state in Ga1−xMnxAs gives us a starting
point from which to describe the nature of ferromagnetic interactions in this DMS. An excellent outline of different kinds of magnetic interactions is given in the Jungwirth
et al. review article []. I will summarize here the essentials of these mechanisms, since that is necessary to put the interactions actually involved in Ga1−xMnxAs
ferro-magnetism in perspective.
1. magnetic dipole-dipole interaction. The interaction strength between two mo-ments separated by a lattice constant is estimated by Jungwirth et al. to be ∼ 1 K, or 10−4 eV. This is weak enough to be unimportant for generating
ferromagnetic order. See also section 1.2.
2. spin-orbit coupling. The spin of an electron interacts with the effective magnetic field resulting from its orbital motion [[54–56]]. This effect is very important for magnetic anisotropy, but generally not important for onset of magnetic order.
overlapping charge distribution []. This change in overlap changes the energy of the resulting state is a way that is dependent upon spin orientation.
(a) direct exchange (Heisenberg) This is simply an exchange interaction as de-scribed above, occurring between two local spins and corresponding to the energy difference between a symmetric and and antisymmetric orbital wave-function.
(b) itinerant exchange (Stoner) Parallel spin polarization of itinerant (delo-calized) charge carriers reduces wave function overlap, reducing repulsive interactions between charges. However, this effect competes with the band energy minimization that occurs by doubly occupying each Bloch state (which can only happen with paired spins). If the system has a large den-sity of states at the Fermi energy, spin polarization can cost very little kinetic energy while saving exchange interaction energy. Since itinerant ex-change by definition applies specifically to delocalized spins that are part of band structure, this effect is not the major one driving the ferromagnetism in III1−xMnxV DMS, which have localized Mn spins.
(c) superexchange (Kramer) In this case one has a system of local moments separated by a non-magnetic atom. When an electron is transferred from the nonmagnetic to the magnetic atom, it interacts via direct exchange with the local moment of the magnetic atom. The non-magnetic atom, coupled to all of its neighbors, therefore becomes polarized to some degree. So superexchange proceeds as the net effect of two direct exchange inter-actions, and their relative sign determines whether the superexchange is ferromagnetic or antiferromagnetic.
electrons hopping through the intermediate non-magnetic atom. The net effect is a ferromagnetic interaction, because
i. Hund’s rules [] indicate that the lowest energy in partially-filled shells is achieved by parallel spin alignment, and
ii. parallel spin alignment decreases the magnetic electrons’ kinetic energy by increasing the hopping probability.
Double exchange most likely to be important at low Mn doping and in wide bandgap materials.
(e) kinetic exchange; indirect exchange (Zener) This exchange mechanism is basically the weak coupling limit of Zener’s double exchange. In this case, rather than propagating via tightly-bound carriers that hop between the localized magnetic moments (double exchange), the effective exchange be-tween localized magnetic moments is mediated by delocalized charge carri-ers. The net exchange interaction between local moments is ferromagnetic when the charge carriers are associated with the local moment site, and it is antiferromagnetic when this effect results from hybridization between the local moment and charge carriers on neighboring sites. The delocalized nature of the charge carriers automatically carries this exchange interaction to multiple localized moments.
A distinction is also often made between effective exchange and direct exchange (3a). Effective exchange refers to an interaction that occurs between magnetic moments that don’t overlap directly, and typically can be described as a sequence of direct exchange interactions. Therefore the term effective exchange is meant to encompass every kind of exchange on the above list other than direct exchange.
Zener’s indirect exchange, 3e, sometimes referred to as kinetic exchange, is the mechanism that applies most directly to ferromagnetism in Ga1−xMnxAs. The
accep-tor nature of MnGa ensures that not only are the localized 3d Mn spins present, but
levels at the top of the valence band are more strongly associated with the As sub-lattice (see discussion of GaAs bond ionicity on p. 24), which means they are limited in their overlap with the Mn d electrons, weakening the direct exchange between the 3d spins and the 4s holes. In this case the dominant interaction is instead antiferro-magneticp–d hybridization []. Hybridization is nothing other than the energy level repulsion of similar electron states; it is the same thing that creates band structure in the first place, and it is often described mathematically in quantum mechanics by taking linear combinations of non-interacting orbitals. In this case we can understand the effect qualitatively by expecting that the states with like spin will “repel” each other. Given filled, down Mn levels deep in the valence band, and unfilled, spin-up Mn levels high in the conduction band, such level repulsion will split the energy of the 4p valence band by spin, raising the energy of the spin-down valence states and lowering the energy of the spin-up valence states. It is clear that this interaction is antiferromagnetic, since lowering the energy of the spin-down 4p states relative to the Fermi level means creating a majority spin band of charge carriers with opposite spin from the Mn 3d band.
Defects That Detract From the Ferromagnetic Properties
There are two primary ways in which defects in Ga1−xMnxAs can reduce the overall
strength of ferromagnetic interactions. Charge compensation can lower the density of charge carriers in the material, which weakens the ferromagnetic state since the charge carriers mediate the itinerant exchange. In the present case of p-type conductivity, this refers to unintentional donor defects that donate excess electrons to the crystal. Magnetic defects that interact antiferromagnetically with the localized Mn moments also destabilize the ferromagnetic state. Both kinds of defects have the net effect of lowering TC, so understanding what they are and minimizing their effects is key to
maximizing TC in Ga1−xMnxAs.
The As antisite defect, AsGa, is already familiar from the discussion of defects in
content, so this defect was particularly prevalent in LT-MBE-grown samples [[41–43]]. Because Ga1−xMnxAs requires nonequilibrium LT-MBE growth conditions, it is likely
to suffer the same difficulty. Since AsGa consists of a Group-III element on a Group-V
site, AsGa is a double donor, compensating the MnGa acceptors.
The other major defect in Ga1−xMnxAs is the Mn interstitial defect, MnI [].
Since MnI is not actively involved in the bonding, but it gives up its 4s electrons
readily, it acts as a double donor in Ga1−xMnxAs, compensating the MnGa electrically.
Although in an as-grown sample with x=0.09 approximately 17% of the Mn was measured to be incorporated as MnI [], it was determined that low-temperature
annealing decreased the observed compensation significantly. Subsequent attempts at monitoring the annealing even more carefully and carrying it out at lower temperatures resulted in a considerable increase in TC, up to 140 K from the previous limit of
110 K []. Further study revealed that the annealing caused MnI to diffuse towards
the open surface of the film and become passivated at the surface []. While the activation energy for diffusion of MnGa in GaAs was determined to be 2.75 eV [], it
is estimated to be only 1.4 eV for out-diffusion of MnI[[46,60]]. This energy separation
permits low-temperature annealing to remove MnI without disturbing the MnGa.
MnI that is in registration with the zinc blende lattice [] could be surrounded
by either a tetrahedral arrangement of either Ga (TGa) or As (TAs) [[60, 61]]. When the MnI is fully ionized, it has given up both 4s electrons to become MnI2+. Although
the ionicity of the GaAs host crystal has been debated [], it nevertheless must lie somewhere between the ionic limit, Ga3+As3−, and the covalent limit, Ga−As+.
More recently, experimental and theoretical results have converged upon the expected consensus: there is a small net transfer of charge to the As [[62, 63]]. This means that we would expect the Coulomb force to lower the energy of an MnI2+ slightly in a TAs
location relative to that in aTGa location []; other calculations [] indicate that in
compensated Ga1−xMnxAs neither site is preferred, and in p-type material, the TGa
believe that an MnI2+ can be further stabilized if it is located next to a substitutional
Mn site, MnGa, where the MnGa acts like a group II acceptor and is negatively charged
on average [[60, 61]].
Calculations by the same groups [[60, 61]] also indicate that the MnI interacts
anti-ferromagnetically with the MnGato which it is bound, acting to neutralize its magnetic
properties. Experimental results also demonstrate this antiferromagnetic interaction before annealing []. Therefore it is understood that the dramatic increases in TC
achieved upon annealing (for example TC = 55 K to TC = 145 K []) as a result of
MnI out-diffusion are not merely due to increasing ρh, but are also due to magnetic
re-activation of MnGa.
Although AsGa is expected to contribute to charge compensation of MnGa, and
almost certainly did play a role in early Ga1−xMnxAs sample TC’s, AsGa is immobile
in the lattice below a temperature of 450–500◦C [[43,46]]. Since Mn
Ga becomes mobile
at a much lower temperature (annealing temperatures achieving the highest TC are
190◦C []), researchers seem to be stuck with the amount of As
Ga that is initially
grown-in. However, growth using As2 instead of As4 [], as well as careful control
of stoichiometry [], can result in films with no detectable electrical compensation from AsGa [].
words, the formation energies of AsGa and MnI, both donors, decrease with increasing
concentration of the desirable MnGa acceptor. A large concentration of either donor,
AsGa or MnI, will suppress the formation of the other donor defect. These theoretical
calculations explain very well the observed increase in MnIthat inevitably accompanies
increases in x for Ga1−xMnxAs [].
Curie Temperatures in Ga1−xMnxAs
As indicated in the section on defects in Ga1−xMnxAs, starting on page 15,
under-standing the nature of defects in Ga1−xMnxAs has been the key to improvingTCin the
samples. Ohno et al.[] started out with a maximum TC = 60 K for a Ga1−xMnxAs
sample withx= 0.035. Two years later Ohno [] reportedTC = 110 K forx= 0.053.
After this report, though, nearly four years passed before any significant increases in
TC were made [].
Researchers reported the potential for TC improvement through low temperature
annealing [[69, 70]]; and Edmonds et al. finally broke the 110 K barrier in 2002, pro-ducing a TC = 140 K sample with x = 0.06 by careful resistance monitoring of the
annealing process. In a later paper Edmonds et al. [] demonstrated conclusively that MnI diffusion towards the sample surface was responsible for the increase in
con-ductivity and for the increase in TC. Their data showed that the dominant cause of
the conductivity change is an increase in ρh, and that µh changes are minor.
The current record for TC is TC = 173 K [], for a sample with x = 0.09 total
Mn content as measured by SIMS, but for whichx= 0.068 was the amount estimated to be active after annealing, or not magnetically decoupled by nearby MnI. Thus far
experimental results for high-quality films are consistent [] with the Zener model of itinerant exchange that was proposed by Dietl et al. [] for zinc blende DMS, which predicts that TC ∝ xρ1/3h . In other words, there seems to be no fundamental
limit to increasing TC in Ga1−xMnxAs other than the considerable difficulty involved
The magnetic moment µ per MnGa in Ga1−xMnxAs is found to be in the range
of 4–5µB [], taking into account the fairly large uncertainty in the measurements.
Arriving at these numbers involved performing electrical measurements to identify the MnGa and MnI concentrations, and assuming that each MnI removes one MnGa from
the active Mn fraction. Magnetic moment peractive MnGa was reported, rather than
per nominally-introduced Mn. (Magnetization per nominally-introduced Mn for the annealed material, including both MnGa and MnI, was instead in the 3–4µB range.)
This result, consistent over a range of films with nominal Mn concentrations ranging from x = 2.2–8.4%, agrees precisely with the saturation magnetization of 4.5–4.7µB
predicted by theory. Although the magnetic moment of an individual MnGa would be
5µB because of the 3d5 electrons, this moment is reduced slightly through
antiferro-magnetic coupling with the 4p band holes []. While Ohno et al. [] had already reported a magnetization of approximately 4.4µB per Mn in their original growth of
Ga1−xMnxAs, without any annealing and using the nominal Mn concentration for the
calculation, in light of the above results this has to be regarded as a coincidence.
Lattice parameters in Ga1−xMnxAs
There has been some contention over the dependence of the lattice constant in Ga1−xMnxAs on the various impurities, both intentional (MnGa) and unintentional
(MnIand AsGa). For example, some DFT (density functional theory) calculations []
indicate that the increase in lattice constant in Ga1−xMnxAs is almost exclusively due
to MnI and AsGa defects. This would appear to agree with the typically-observed
trend of increasing lattice constant with increasing Mn doping, since concentrations of MnI and AsGa increase along with MnGa (see the discussion of self-compensation
beginning on page 25). However, careful measurements [] indicate that although MnI and AsGa do contribute to the observed lattice expansion, the MnGa does in fact
provides a more detailed discussion and additional references.
Magnetocrystalline anisotropy is the dependence of a ferromagnet’s free energy on the angular orientation of its magnetic moment. This should be expected, especially in the case of ferromagnetism mediated by itinerant exchange (see the section on exchange interactions beginning on p. 20), where the communication between the spins happens by virtue of the valence band holes []. From the point of view of any individual spin, the angular dependence of the surrounding hole density (responsible for mediating the magnetic interactions) reflects that of the band the holes reside in. Formally we say that the anisotropy in Ga1−xMnxAs originates from spin-orbit
coupling in the valence band [].
While one might at first expect this anisotropy simply to reflect the underlying cubic structure of the GaAs host crystal, there are several additional sources of uniaxial contributions to the anisotropy.
1. Boundary conditions from Maxwell’s equations result in a “shape anisotropy” which creates a preference for the spins to align parallel to the surface of the thin films.
2. On any of the crystal faces, the cubic symmetry of the bulk zinc blende crystal is broken across the diagonal of the cube face. See Figure 2.1 on page 13. This surface effect can cause an in-plane uniaxial contribution to magnetic anisotropy in zinc blende materials.
3. Finally, any strain present in the material can result in a uniaxial anisotropy contribution along that direction, due to the inverse magnetostriction effect.
It turns out in Ga1−xMnxAs that effects due to strain dominate the anisotropy.
generally lie in the plane of the film, the (001) plane, as would be expected due to shape anisotropy, this is better-understood to be a result of biaxial strain in the Ga1−xMnxAs epitaxial layer [[76,77]]. This strain originates from the lattice expansion
discussed above beginning on page 27, which is responsible for a lattice mismatch between the GaAs substrate and the Ga1−xMnxAs DMS film. This expansion means
that Ga1−xMnxAs grown on a GaAs substrate experiencescompressive strain. Biaxial tensile strain is typically achieved by growing the Ga1−xMnxAs on top of an GaInAs
film, and results in an out-of-plane easy axis.
Many different groups have characterized the magnetic anisotropy in Ga1−xMnxAs
/ GaAs via a variety of methods, and have found the following results. Some observe that the easy axes always lie in the in-plane h100i directions [[78, 79]] as a result of dominant cubic anisotropy. Others observe that the easy axis starts out in the in-plane h100i directions at low temperature, accompanied by a small uniaxial anisotropy that makes the in-plane h110i directions inequivalent. As the temperature increases the cubic anisotropy term decreases in magnitude relative to the uniaxial term, such that at higher temperatures the  axis becomes the easy axis [[80–82]]. Finally, some report a uniaxial easy axis along the  direction []. It seems clear that these reports of anisotropy are qualitatively consistent.
The inequivalence between  and£110¤directions is not yet fully understood. It evidently does not result from the most apparent potential sources of in-plane uniaxial anisotropy. Welp et al. demonstrated [] that the in-plane uniaxial anisotropy was independent of film thickness, and Sawicki et al. [] further showed that etching away as much as 50% of the annealed Ga1−xMnxAs layer had no effect. These results
therefore present throughout the entire thickness of the film.
Sawicki et al. [] performed a set of careful measurements of both the cubic and in-plane uniaxial anisotropy contributions under varying temperatures and hole densities ρh, and mapped out the dependence of the easy axis orientation on these
parameters. They found the easy axis could point in either the (in-plane)h100i, , or£110¤directions depending on conditions. Furthermore they were able to model the observed magnitude of and temperature andρh dependence of the magnetic anisotropy within the Zener model of itinerant exchange, after introducing a phenomenological trigonal distortion (shear strain ²xy ≈5%).
There is much less to say in the review of Ga1−xMnxN materials properties, mostly
because much less is understood about this material. Ga1−xMnxN is, of course, a DMS
based on GaN, which is a wide-bandgap (∼3.4 eV) III-V semiconductor. Dietl, Ohno, and Matsukura generated a great deal of interest in Ga1−xMnxN as a potential solution
to theTCproblem by publishing theoretical papers [[71,85]] that predicted, among other
things, aTCfor ferromagnetic Ga1−xMnxN (x= 0.05,ρh = 3.5?1020holes·cm−3)
signif-icantly above room temperature. Subsequent attempts at growth and characterization of Ga1−xMnxN have given widely varying results, ranging from TC = 10 – 20 K [],
to 220 – 370 K [], to 940 K [[88, 89]]. The range of variation in the results has not been explained satisfactorily; and claims of above-room-temperature ferromag-netism have not been met with widespread acceptance [[90, 91]]. Furthermore, mate-rials for which TC was measured to be above room temperature have generally been n-type rather thanp-type, so the model behind the Dietl et al. prediction [[71, 85]] for
p-type Ga1−xMnxN cannot apply. In fact, it has proven so difficult to grow p-type
Ga1−xMnxN that it seems likely that this particular high-TC prediction will never be
evaluated directly [].
of GaxMny or MnxNy are not present and responsible for the observed magnetic
prop-erties [[90, 92]]. If the predominant phase of Ga1−xMnxN is not ferromagnetic at the
experimental temperature, the magnetic response of a ferromagnetic secondary phase, present even in very small quantities, could easily dominate the experimental results. X-ray diffraction (XRD) is the most common way to determine the bulk structure of a sample, but it is not particularly well-suited for detecting small deposits of secondary phases, since the signal strength and peak width from tiny crystallites is directly related to their size and quality.
It is not immediately obvious that ferromagnetism resulting from secondary phases would be undesirable, especially if those phases or clusters of atoms were so small and well-dispersed as to be undetectable by XRD. However it is at least likely that such ferromagnetism, resulting from small embedded clusters of material that is otherwise ferromagnetic in bulk, does not depend on or interact much with the host GaN crystal or band structure. In that case, not only are well-understood Zener itinerant exchange models completely inappropriate for describing the magnetic materials properties, but also low polarization of the charge carriers would be likely. Low charge carrier polarization is undesirable for implementing spintronic devices.
Structural Characterization of
Raman scattering is one of the two primary, complementary methods for mea-suring vibrational modes of materials (the other primary method is infrared, or IR, absorption). Since Raman scattering involves the inelastic scattering of light from phonons, it can be considered to be a three-body interaction involving an incident photon, with angular frequency ωphotI, and wavevector kI; a scattered photon with
angular frequency ωphotS, and wavevector kS; and a phonon with wavevector q. As
phonons either created or annihilated in this interaction, it is strictly necessary to treat the phenomenon of Raman scattering within the quantum-mechanical frame-work known as second quantization. However, a straightforward semiclassical model of the Raman effect explains many of its features in an exceptionally clear manner.
χe, connects the electric polarization
P and the electric field ˜
E as follows:
P = ˜˜
χeis a tensor which obeys certain symmetry considerations depending on the symmetry
of the material (see Nye []). This macroscopic description of Raman scattering will follow closely the presentation in Yu and Cardona [].
The presence of a phonon will modulate ˜˜
χe at the frequency of the phonon, ωphon,
which can be expressed by performing a Taylor expansion of ˜˜
χe as a series in
Q( ˜r, t), the lattice wave of atomic displacements.
˜˜ χe ¯ ¯ ¯ 0
∂ ˜ Q ¯ ¯ ¯ 0 · ˜ Q(
˜r, t) +. . .
= ˜˜ χe ¯ ¯ ¯ 0
∂ ˜ Q ¯ ¯ ¯ 0 · ˜ Q¡
+. . .
This expansion is carried out by making the quasistatic approximation, which amounts to saying that the time variation of
˜r, t) is slow compared to the electronic response time. Therefore
˜r, t) acts like a static polarization from the perspective of χ˜˜e. Combined with the electric field from the incident light, oscillating at a frequency of
ωphotI, we get:
P = ˜
∂ ˜ Q ¯ ¯ ¯
¢ · ˜ Einc ¡ ˜
kI, ωphotI¢cos¡ ˜
1 2 ∂ ˜˜ χe ∂ ˜ Q ¯ ¯ ¯ 0 · ˜ Q¡
¢ · ˜ Einc ¡ ˜
. ..ncos¡£ ˜
ωphotI+ωphon0¤t¢+ cos¡£ ˜
ωphotI−ωphon¤t¢ o ,